Photovoltaic Module Weather Durability & Reliability http://us.sunpower.com
Weather Durability &
Will my module last outdoors?
Allen F. Zielnik
David P. Dumbleton, Ph.D.
Solar Energy Competence Center
Atlas Material Testing Technology LLC
The information contained in this document is the proprietary and exclusive property of Atlas
Material Testing Technology LLC except as otherwise indicated. No part of this document, in
whole or in part, may be reproduced, stored, transmitted, or used for design purposes without
the prior written permission of Atlas Material Testing Technology LLC.
The information contained in this document is subject to change without notice.
The information in this document is provided for informational purposes only. Atlas Material
Testing Technology LLC specifically disclaims all warranties, express or limited, including, but not
limited, to the implied warranties of merchantability and fitness for a particular purpose, except
as provided for in a separate software license agreement.
Atlas Material Testing Technology LLC
4114 N. Ravenswood Avenue
Chicago, IL 60613 USA
Phone +1 773.327.4520
Fax +1 773.327.5787
Table of Contents
Business Challenge ……………………………………………………………… ... …..4
What Is Known………………………………………………………………….…..……..5
Reliability and Durability………………………………………….………...…………...6
IEC Qualification Tests…………..……………………………………………...............8
Accelerated Testing………………………………………………………………. .…….9
Photovoltaic Module Weather Durability and Reliability Page 2 of 17
Most manufacturers of solar modules guarantee the minimum performance of their modules for 20 to
25 years, and 30 year warranties have been introduced. The warranty typically guarantees that the modules
will perform to at least 90% capacity in the first ten years and to at least 80% in the remaining 15 years.
Even though the hardware warranty may be shorter, the economics are based on the longer term.
Under most general accounting practices, manufacturers are obliged to set up reserves for the expected
volume of claims under the performance warranties. The result is that the capital tied up in the reserves is
no longer available for investment. However, reserves mostly cover only some of the liabilities that arise in
the event of a loss – serial losses often affect several production years. A single serial loss could be sufficient
to threaten a module manufacturer’s existence and market position.
Early life failures resulting from design flaws, materials or processing issues are often apparent during the
first few years in service. The requisite design qualification and approval tests such as IEC 61215 for
crystalline silicon and IEC 61646 for thin films are relatively short accelerated tests which attempt to discover
these early “infant mortality” issues. Safety tests, such as UL 1703/IEC 61730, are performed only on new
modules and tell little about safety performance after long-term field exposure.
More importantly, many module failures and performance losses are the result of gradual accumulated
damage resulting from long-term outdoor exposure in harsh environments, referred to as “weathering”. Many
of these processes occur on relatively long time scales and the various degradation processes may be
chemical, electrochemical, thermal or mechanical in nature. These are initiated or accelerated by the
combined stresses of the service environment, in particular solar radiation, temperature and moisture, and
other stresses such as salt air.
Weatherability testing has been successfully relied upon by industries such as automotive, building products,
polymers, paints and protective coatings for over 90 years. Much has been learned about materials
degradation and proper accelerated weathering approaches in that time. Weathering tests for longer term
degradation are very different from the “infant mortality” stress tests that are used in the IEC standards, even
when run for longer periods of time.
The Atlas Solution
Atlas, the recognized global leader in weatherability testing, has developedAtlas 25PLUS, a comprehensive,
multi-dimensional, environmental weatherability program for PV modules. A complement to the IEC
“infant mortality” tests, this one-year program delivers the weathering stresses representative of long-term
outdoor exposure otherwise unattainable without lengthy real-time testing. Independent 3rd party data from
Atlas 25PLUS supports your product R&D and cost reduction efforts, supports your warranty and
performance claims, and provides validation to financial stakeholders at all levels.
Photovoltaic Module Weather Durability and Reliability Page 3 of 17
Importance of PV Module Economic Performance
Apart from government financial credits and incentives, the economics
of photovoltaic (PV) systems of all sizes is based on their reliability to
deliver the rated power over their expected service lifetime. Financial
penalties result when modules prematurely fail during the hardware
repair or replace limited warranty period (typically 1 – 10 years), when
unanticipated service or maintenance is required, or when power
delivery falls to unacceptable levels. Today, this performance warranty
is frequently >90% of rated power after 10 years and >80% after 20 or 25
years although 30 year guarantees have now appeared with 40 years
being anticipated soon.
The real issue then becomes, how can we guarantee 20 or more years
when most current module designs and technologies have only a few
years or less of field history? What predictive tools are available and
what is our confidence in them? The answer has major implications for
all financial stakeholders: venture capital for new product R&D; OEM
warranty set-aside reserves; bank financing of PV systems; system
insurers; and end users/system owners.
How can we
guarantee 20 or
more years when
have only a few
years or less of
The Need for Accelerated Tests
John H. Wohlgemuth of BP Solar describes the fundamental problem:
“Outdoor testing is a must, but it takes much too long to be of much use
as a decision maker. We clearly can not wait 25 years or even a significant
fraction of 25 years to introduce a new product. Therefore, we must
develop and utilize accelerated tests to qualify these new products.”1
Akira Terao, Chief Reliability Engineer for Sunpower Corporation goes
further to identify some of the life-testing roadblocks:2
25 year warranty
Ill-defined field conditions
Harsh and varied outdoor conditions
Materials used near their limits
Limited acceleration factors ⇒ long tests
Large samples, small sample sizes
Subtle polymer chemistry
Cumulative effects, positive feedback loops
Clearly, assessing PV module lifetime performance is not a simple task.
1John H. Wohlegemuth, et al, “Long Term Reliability of Photovoltaic Modules”, 23rd EU PVSEC Conference, 2008
2Akira Terao, “Modules: Remaining Reliability Challenges”, Accelerated Aging and Reliaibility in PV Workshop, 2008
Photovoltaic Module Weather Durability and Reliability Page 4 of 17
What Is Known?
PV Module Reliability and Durability Concerns
If a module fails to generate power it is an obvious failure and a reliability issue.
However, environmental degradation such as corrosion can cause a gradual
decrease in power output which is a durability issue (or more precisely, a lack of
durability). Durability issues may also eventually lead to module failure.
Dr. Sarah Kurtz of the U.S. Department of Energy’s National Renewable Energy
(NREL) PV module reliability group maintains an on-line living document of known
reliability/degradation issues for PV modules. “General reliability
issues across all PV technologies are:
1.Corrosion leading to a loss of grounding
2.Quick connector reliability
3.Improper insulation leading to loss of grounding
6.Bypass diode failure
“In addition there are issues specific to the individual technologies, to name a few:
I.Wafer silicon: Light‐induced cell degradation, front surface soiling, effect of glass on
encapsulation performance, reduced adhesion leading to corrosion and/or
delamination, busbar adhesion degradation, junction box failure
The majority of
these issues is
II.Thin Film Silicon: Electrochemical corrosion of SNO2, initial light degradation
III.CdTe: Interlayer adhesion and delamination, electrochemical corrosion of SnO2:F,
shunt hot spots at scribe lines before and after stress
IV.CIS: Interlayer adhesion, busbar mechanical adhesion and electrical [integrity],
notable sensitivity of TCO [transparent conducting oxide] to moisture, moisture
ingress failure of package
V.OPV: Photolytic instability, moisture induced degradation, moisture ingress failure of
The majority of these issues is either directly caused or influenced by outdoor in-
service environmental exposure; therefore the need to accelerate and study the
effects of weather and climate on PV durability and reliability is crucial.
3 Dr. Sarah Kurtz, National Renewable Energy Laboratory, “Reliability Concerns Associated With PV Modules ”,
Photovoltaic Module Weather Durability and Reliability Page 5 of 17
Reliability & Durability
Reliability Engineering in Photovoltaics
Reliability engineering is a structured discipline which concerns itself primarily
with absolute, discrete failures, their detection and statistical measurement such
as Mean Time To Failure (MTTF), Mean Time Between Failures (MTBF), number
of failures per nnumber of units and similar measurements. The methodology
requires statistically high numbers of samples, preferably from production lots.
Therefore, statistical methods cannot be used on limited R&D prototypes.
Testing techniques such as highly accelerated life testing (HALT) are widely
employed in reliability (failure) analysis by PV manufacturers and other
industries. Gregg K. Hobbs, the inventor of HALT and HASS (highly accelerated
stress screening), points out several key limitations of HALT which are often
“HALT does not
simulate the field
only seeks to find
process flaws by
- Gregg K. Hobbs
Inventor of HALT testing
HALT does not attempt to simulate the field environment ‐ only seeks to find
design and process flaws by any means possible.
Intent is to determine failure modes, NOT demonstrate that a product meets
Not meant to determine reliability but to improve it.
Test environments are not directly related to real life and may be controversial.
Time‐dependent failure modes may not be revealed.
Difficult to do on complex structures because of complex loading – FMVT
(failure mode verification testing).
Another critical aspect of HALT testing is that correlation does not prove
causation. In other words, just because you obtain a result (change or failure) in a
HALT test that seems to match that from the real time field use doesn’t prove it
was caused by the same mechanisms. Cause and effect must be proven.
Further, HALT testing works best for accelerating physical degradation modes
and may be incapable of accelerating chemistry-induced degradation.
Durability testing on the other hand, when applied to studying the degrading
influences of outdoor environmental stresses (known as weathering) is a highly
specialized interdisciplinary science that is concerned with:
routes to failure (mechanisms)
rates of property change (performance)
stress‐stress interactions (synergy)
simultaneous and sequential degradation process
These concerns may affect critical performance properties or lead to outright
failure; evaluating the effects of various climates on product performance and
life is a core aspect of product weatherability assessment.
4 Gregg K. Hobbs, “Accelerated Reliability Engineering: HALT & HASS”, John Wiley & Sons
Photovoltaic Module Weather Durability and Reliability Page 6 of 17
Durability, Reliability and the Bathtub Curve
Another way of considering durability v. reliability and HALT v. weathering is
through the classic “bathtub reliability curve” describing failure rate as a function
of in-service life. Early-life failures, referred to as “infant mortality,” typically
occur out of box into the first 1–2 years of a product’s life. These may result from
fundamental design flaws but also from materials or processing issues. Remember,
short-term HALT-type testing is subject to the limitations Hobbs addresses.
testing focuses instead on
the longer term in-service
period. This is the period
where the time-
application of combined
delivered in their natur
short and long-term
cycles, causes degradation and accumulates damage which causes wear-out and
eventual failure. In this accumulated damage model no single stress-relaxation
event will cause failure, but the accumulated damage resulting from long-term
exposure will lead to decreasing performance
and eventual failure.
As multiple simultaneous and/or sequential degradation mechanisms may be at
work in long-term exposure, failure often is the result of prior events (accumulated
damage) that HALT does not adequately address. For example, an elastomeric or
polymeric module edge seal may become brittle from UV and thermal degradation
leading to moisture ingress producing internal corrosion of the transparent
conducting oxide (TCO) layer visible as module discoloration resulting in electrical
These overlapping and/or sequential degradation modes (illustrated below) can
interact to produce module failure. Basic HALT tests cannot reproduce the
complex stress interactions of the real-world environment as illustrated below:
often results from
the interaction of
basic HALT tests
Photovoltaic Module Weather Durability and Reliability Page 7 of 17
IEC Qualification Tests
IEC Design Type Qualification Tests
Photovoltaic module designs must be tested in accordance to IEC 61215 for
wafer based silicon and to IEC 61646 for thin film technologies. A summary of
the key environmental-related tests within the larger IEC 61215 regimen (IEC
61646 is similar) is shown:
It is important to note several aspects of this protocol (the exact test parameters are
in the IEC documents):
No single module goes through the full complement of environmental tests
No simultaneous solar radiation, temperature and humidity stresses as outdoors
The test parameters (temperature, humidity, etc.) are more extreme than and not
representative of any real climate
No test (except for a short outdoor exposure) is under full solar radiation
Chamber tests do not combine solar radiation, temperature, and humidity as in
Short test durations and low cycle counts (e.g., 200 thermal cycles or 1,000 hours
damp heat each take only about 6 weeks to run)
PV modules are not electrically active (light bias) during exposure
“… the relatively
short tests in the
standards do not
and cannot provide
lifetime data …”
The IEC qualification tests are HALT-type tests which focus on short-term “infant
mortality” resulting from design, materials and processing defects. They do not
imply any longer term life or climate-specific performance but only serve as a
minimum commercial requirement.
NREL and ASTM
It is important to note that extending these tests to longer durations or additional
cycles, while useful for forcing and identifying some potential failure modes
(subject to Hobbs’ limitations), do not provide the predictive natural weathering
stresses required in weathering testing. The previous lack of suitable large-scale
accelerated weathering chambers to accommodate full size PV modules has largely
limited testing to this inadequate approach or to using non-representative mini-
module samples in conventional weathering tests. Atlas 25PLUS overcomes these
limitations. As you can see, neither HALT nor IEC tests are suitable for producing
Photovoltaic Module Weather Durability and Reliability Page 8 of 17
Accelerated Photovoltaic Testing
Carl Osterwald and Tom McMahon of NREL published an exhaustive and well
annotated review of PV module testing since 1975 leading up to the development of
the IEC and related tests. They note the limitations and the need for improved
methods, especially in the area of long-term durability testing: “The intent and
history of these qualification tests, provided in this review, shows that standard
module qualification test results cannot be used to obtain or infer a product lifetime.
Closely related subjects also discussed include: other limitations of qualification
testing, definitions of module lifetime, module product certification, and accelerated
Accelerated Weathering Testing
Formal outdoor weather exposure testing has a hundred year history. While
necessary, the lengthy times required for real-time testing are a hindrance to new
product development and introduction for all long-lived products. As a result,
accelerated weather testing, pioneered by Atlas in 1915, has been in continuous
development for 95 years. Today, both accelerated outdoor and laboratory
accelerated weathering are essential in industries such as automotive, military,
aerospace, building products, polymers-paints-coatings, and materials science. They
have been widely applied to solar energy materials and products since Atlas first
tested the PV modules used for the original Skylab launched in 1973 and are used by
materials suppliers, PV manufacturers and laboratories such as NREL.
Laboratory-accelerated weathering is a specialized form of Accelerated
Environmental Testing (AET). While oven aging, UV exposure or thermal-cycling
chambers are various forms of AET, laboratory accelerated weathering has a specific
set of minimum requirements, notably:
easy . . . lifetime
Full‐spectrum simulation of terrestrial solar radiation (AM1 to
Control of chamber air temperature
Monitoring of test specimen or reference panel temperature
Control of relative humidity
Simultaneous cycling of solar Irradiance, air temperature and
Akira Terao -
While materials-level or small-scale product tests are usually performed at above-
ambient temperatures (under steady-state or cycling conditions), the complex multi-
layer laminate structure of PV modules requires a wider range of environmental
control to simulate real climatic conditions.
5 History of Accelerated and Qualification Testing of Terrestrial Photovoltaic Modules: A Literature Review, ©2008,
Photovoltaic Module Weather Durability and Reliability Page 9 of 17
Weathering Testing of Full Scale PV Modules
Due to module size and the prior lack of suitably large accelerated weathering
devices, apart from real-time outdoor testing the best approach has utilized small
(typically 1-cell) “mini-module” test specimens in standard-sized commercial
weathering instruments. This “mini” test approach has several key limitations.
First, mini-module test specimens typically do not go through normal production
equipment. Secondly, their down-sizing produces mechanical stresses such as
those resulting from thermal expansion; these may be very different than that of full
sized modules. Third, most standard accelerated weathering instruments for small
samples lack the full cycle temperature ranges (especially at the low end) that
modules will encounter. And finally, no standard or custom accelerated weathering
chamber can deliver all of the natural stresses which are likely to be encountered,
such as salt air corrosion in combination with temperature, humidity and solar
As a result, Atlas has pioneered new state-of-the-art accelerated weathering
chambers such as the XR360™ and SolarClimatic 2000 to expose full size PV
modules which is a cornerstone of Atlas 25PLUS testing.
Photovoltaic Module Weather Durability and Reliability Page 10 of 17
Atlas 25PLUS Program
Atlas 25Plus PV Module Durability
Given the critical industry need and the lack of module-suitable accelerated
weathering methodologies, Atlas has drawn on 90 plus years of weather testing
experience, with more than 25 of them in PV and solar materials, to develop the
Atlas 25PLUS PV Module Durability Testing Program. Unlike IEC type design
qualification tests which target early-life failures, Atlas 25PLUS targets the long-term
effects of weather and climate that modules will experience in service to provide
critical lifetime and performance data to support manufacturer’s claims.
Atlas 25PLUS leverages the key research findings on degradation across all
photovoltaic technologies as well as advanced weathering testing techniques.
Atlas has developed new accelerated weathering instruments, such as the
XR360™ large-scale weathering chamber, to expose full size modules.
Atlas 25PLUS does not duplicate the IEC or similar tests. Atlas 25PLUS does
generate independent third-party data for manufacturers to both improve
product reliability and performance and provide best-available assurance to
Atlas 25PLUS neither duplicates nor replaces IEC qualification testing, but rather
is an essential complement to help answer the question, “Will my module last
A comparison of “qualification testing” and Atlas 25PLUSillustrates the
Photovoltaic Module Weather Durability and Reliability Page 11 of 17
Core Concept of Atlas 25PLUS
Nature does not change the way it delivers weather and climate based on your module.
Therefore, Atlas 25PLUS is designed to deliver the key weather and climate stresses, at the
levels found in nature, in both short-term daily and longer term seasonal cycles. This
approach treats your module as a “black box” and while independent of specific PV
technology or design, incorporates the stresses found in nature identified as detrimental
to photovoltaic modules.
Drawing on Atlas’ data and experience, three specific service environments have been
identified as most damaging: hot arid desert, tropical/subtropical and northern
temperate. Modules designed for specific deployment, such as utility-scale systems for
desert locations such as Southwest USA or Middle-East, may optionally be subjected to
one or more of the specific climate simulations. A general “Global composite” climate
based on the worst-case boundary conditions of these three specific harsh climates is
used as the standard exposure condition for products to be used globally as shown in the
Köppen-Geiger climate classification map:
Photovoltaic Module Weather Durability and Reliability Page 12 of 17
Atlas 25PLUS acknowledges the need to balance time-in-test with providing
sufficient stresses representative of long module service life and the limits of
reliable acceleration. Therefore, Atlas 25PLUS takes exactly one year to perform
although interim measurement data is provided throughout the program.
Atlas 25PLUS Weathering Exposures
Three modules are exposed in the standard Atlas 25PLUS base program. One module
is exposed on a solar tracking rack at Atlas’ Solar Test Center in Arizona, and a
second on tracking rack in south Florida. The third undergoes the primary Atlas
25PLUS accelerated aging protocol. Modules are backed similar to a surface roof-
mount to provide elevated but realistic module temperatures.
While under sun or solar simulation, all three modules are exposed operationally
“live” under resistive load for operation at the maximum power point (Pmax). This is
important to stress for electrochemical degradation resulting from ion migration, hot
spots, bypass diode failure, etc. The outdoor tracking exposures provide some
acceleration of two key critically harsh climates as well as benchmark performance
The third module undergoes an initial test sequence:
UV‐A and UV‐B ultraviolet light exposure; provides activation of thin film PV,
Staebler‐Wronski degradation for amorphous thin film silicon, light activation of
inactive semiconductors and photodegradation of polymeric materials
(encapsulants, sealants, potting compounds, cables, Junction‐boxes, topsheets,
backsheets, coatings, etc.)
Salt fog corrosion testing; accelerates marine and alkaline desert metal corrosion
including connectors, micro‐inverters, etc.
Condensing humidity tests; tests moisture ingress into PV, Junction boxes, etc.
This module then
a)Accelerated weathering chamber testing of full‐spectrum solar radiation,
temperature and relative humidity cycling; parameters are climate derived
b)Accelerated weathering chamber cycles of solar, temperature and humidity under
Full-spectrum solar load provides more realistic module stresses than does
basic environmental chamber cycling as well as photodegradation and forward bias.
Photovoltaic Module Weather Durability and Reliability Page 13 of 17
Another key aspect of Atlas 25PLUS is the fast cycle times of the (a) exposure (117 cycles
in 7 days) followed by the (b) cycles (44 cycles in three days). This rapid cycling
provides increased thermo-mechanical stress for greater acceleration. This ten day
core super-cycle is then repeated for a total of 80 days to provide both daily and
seasonal climate-adjusted patterns.
The program then continues with:
Outdoor solar tracking in Arizona for 12 weeks during peak summer
temperature and solar radiation (May, June, July)
Outdoor solar tracking for balance of year (~4 months)
Test cycles and temperatures were designed and tested to target maximum module
temperatures of ~85°C under full spectrum solar radiation. Due to physical size
constraints given the dimensions of most “standard” full sized PV modules, one
module is run through the comprehensive battery, although several smaller-sized
modules may be optionally accommodated.
Measurements and reports
Inspections and measurements are conducted at intervals to characterize module
performance and check for problems. Initial and 12-month final I-V curve
measurements on all modules are taken under our large-scale 1,000 W/m2 near-Class-A
steady-state solar simulator. All interim I-V curves are taken outdoors on days >1000
W/m2 unless optionally arranged.
Visual inspections, digital photographs and digital infrared (IR) thermographic images
are taken at initial, final and 5 interim points. These are approximately every two
months (weather permitting) for the outdoor exposures and at transition points
between chamber test sequences.
Inspection and measurement data is provided as developed during the exposure
permitting qualified exit points in the event of module problems or failures. A final
composite report including these measurements, test site meteorological and solar
radiation data as well as any findings by Atlas is provided at the end of Atlas 25PLUS
As each module manufacturer makes their own determination as to what is acceptable
durability, reliability and performance, Atlas 25PLUS provides no pass/fail criteria or
certification, but does provide data manufacturers can use to provide evidence of their
claims. Completion of the Atlas 25PLUS program allows the manufacturer use of the
What does 1 Year in Atlas 25PLUS Equal?
Atlas 25PLUS is an advanced accelerated weather aging protocol. Precise correlation to
expected performance requires validation with real-time long-term exposure data for
the specific module design. Specific “acceleration factors” for any accelerated test are
highly variable and dependent on materials, product design, manufacturing,
degradation mechanisms and other factors.
Photovoltaic Module Weather Durability and Reliability Page 14 of 17
Acceleration factors and correlation cannot be absolutely predicted without the
requisite long-term outdoor exposure data for the exact module, data which
usually does not exist.
The core Atlas 25PLUS accelerated laboratory exposure is designed to simulate the
key climate stresses such that each cycle provides stresses equivalent to a
minimum of 2 to 5 days outdoors. Additional acceleration is provided by the UV,
condensing humidity, corrosion and solar tracking exposures such that the entire
program delivers exposure equivalents in excess of 10 years real time.
Extending the duration of the core aspects (chamber cycles) of Atlas 25PLUS is
optionally available to increase that confidence level to an expectation of 20 years
Photovoltaic Module Weather Durability and Reliability Page 15 of 17
Value of Atlas 25PLUS
Atlas 25PLUS is the only program designed to answer the basic question of “Will
my module last outdoors?” The answer to this question is crucial to new
product development, to establish warranty and performance claims, and to
provide assurance to financial stakeholders. Failure to understand and
appropriately test for durability to in-service weather and climate risks product
failure and the subsequent financial impact as well as potential safety liability.
Can you answer the question of “Will my module last outdoors?”
For further information contact your local Atlas representative or contact us at
Photovoltaic Module Weather Durability and Reliability Page 16 of 17
Photovoltaic Module Weather Durability and Reliability
Will my module last outdoors?
Authors: Allen F. Zielnik, Dr. David P. Dumbleton
Solar Energy Competence Center
Atlas Material Testing Technology LLC
Copyright ©2010 Atlas Material Testing Technology LLC.
All Rights Reserved, Atlas Material Testing Technology LLC.
All logos, and trademarks or registered trademarks of Atlas
Material Testing Technology LLC or its subsidiaries in the
United States and other countries.
Other names and brands may be claimed as the property of
others. Information regarding third party products is provided
solely for educational purposes.
Atlas Material Testing Technology LLC is not responsible
for the performance or support of third party products
and does not make any representations or warranties
whatsoever regarding quality, reliability,
functionality, or compatibility of these devices or products.
Photovoltaic Module Weather Durability and Reliability Page 17 of 17